The car- boxylic acids citedfor the latter case are not corresponding to those for the former case. constant Alb. Assuming that kl2, k21 Â» k23, Â¿32 in eq 9 and 10,.
Jun 26, 2008 - Densities and apparent molar volumes of aqueous NaH2PO4 (0.1 to 2.1) molÂ·kgâ1, Na2HPO4 (0.1 to 0.5) molÂ·kgâ1 and Na3PO4 (0.4 to 0.6) ...
Jun 26, 2008 - The trisodium phosphate stock solution was prepared by adding a stoichiometric amount of Na2HPO4(s) (Aldrich. ReagentPlus, 99 %), dried at ...
Nov 24, 2014 - ... Technology, TechnickÃ¡ 5, 166 28 Prague, Czech Republic ... Anton Paar DSA 5000 vibrating-tube densimeter and sound analyzer in.
Jan 18, 2013 - sound make possible to evaluate partial molar isentropic com- ...... the Czech Republic (fund MSM6046137307) is acknowledged. Notes.
Jan 18, 2013 - Partial Molar Isentropic Compressions and Partial Molar Volumes of Isomeric Butanediols at Infinite Dilution in Water at Temperatures T = (278 to 318) K and Atmospheric Pressure. LubomÃr HnÄdkovskÃ½ and Ivan Cibulka*. Department of P
Apr 2, 2012 - tube densimeter and sound analyzer in the temperature range ...... the Czech Republic (fund MSM6046137307) is acknowledged. Notes.
Apparent Molar Volumes and Standard Partial Molar Volumes of Aqueous Sodium Phosphate Salts at Elevated Temperatures. Genna E. Woolston, Liliana N.
May 28, 2014 - Density and speed of sound data for dilute aqueous solutions of two crown ethers, 15-crown-5 and 18-crown-6, were measured using the Anton Paar DSA 5000 vibrating-tube densimeter and sound analyzer in the temperature range from (278.15
Macromolecules 1992,25, 4321-4324
Sorption and Partial Molar Volumes of Organic Gases in Rubbery Polymers Yoshinori Kamiya,' Katsuhiko Terada, Keishin Mizoguchi, and Yasutoshi Naito Industrial Products Research Institute, 1-1- 4 Higashi, Tsukuba, Zbaraki 305,Japan Received December 17, 1991; Revised Manuscript Received May 4, 1992
ABSTRACT Sorption of organic gases (CzH4, CzHs, C3H6, C3H8, n-C4Hlo, iso-C4H~o, and n-C5H12)in two rubbery polymers, 1,2-polybutadieneand poly(ethy1ene-co-vinylacetate), and dilation of the polymers due to sorption are measured as a function of gas pressure at 25 "C. Sorption isotherms for all the gases are well described as the Flory-Huggins dissolution. Dilation isotherms are similar i c shape to the corresponding sorption isotherms. From sorption and dilation data, partial molar volumes VR of the dissolved, gases are determined. A linear relation is found between partial molar volume and van der Waals volume_Vw, i.e., TR' = 1.6vw + 18.5 in cm3/mol. This relation is almost the same as that between molar volume and VWfor liquid n-alkanes.
Introduction The knowledge of the thermodynamic state, in particular, the partial molar volume of dissolved gas, has been essential to understand mechanisms of diffusion, sorption, and permeation of gases in polymers.' Recently, the experimental determination of the partial molar volume was done by a few workers.24 They investigated sorption of several gases in polymers and dilation of the polymers due to the sorption, from whose data partial molar volumes of the dissolved gases were determined. However, no clear relationship between the partial molar volumes and the molecular properties of gases has yet been found, because sorption and dilation experiments have not been carried out for any homologous series of gases. To find the relationship is the purpose of the present paper. In this study, we measure sorption and dilation isotherms for organic gases (five alkanes and two alkenes) in two rubbery polymers and determine the partial molar volumes of the dissolved gases. On the basis of the data obtained here and reported p r e v i ~ u s l the y~~ dependence ~ of partial molar volume on van der Waals volume is discussed and compared with volumetric properties of liquid n-alkanes. Experimental Section Materials. The rubbery polymers used are syndiotactic 1,2polybutadiene (PB)(density 0.906 g/cm3) and poly(ethy1eneco-vinyl acetate) (EVAc) (density 0.935 g/cm3,content of vinyl acetate 15wt % ), which are the same as those used previ~usly.~J PB films, ca. 200 pm thick, and EVAc films, ca. 300 pm thick, were employed in both sorption and dilation experiments. Seven organic gases (C2H4, C2H6, C3H6, CsHs, n-C4HlO, isoCIH~O, and n-CbH12) were tested. These gases, supplied by TakachihoChemical Industry, were of at least 99.5% purity and were used without further purification. Sorption and Dilation Measurements. Sorption amounts of gases in a polymer specimen of ca. 200 mg were measured gravimetrically with a microbalance (Cahn Model 2000) placed in a pressure ~ h a m b e r . ~The , ~ microbalance could weigh to a precision of 1 pg under any ambient pressure employed. The magnitude of errorsin sorption measurements was less than f l % of the concentration for all the gases investigated. Dilation isotherms were determined by observing changes in the length of two rectangular film strips (length ca. 60 mm and width ca. 3 mm) suspended in a glass pressure cell.4-5 The two specimens cut in cross directions of the films gave no difference in length elongation within the accuracy of the experiments.For this observation a cathetometer with a precision of 0.01 mm was used, and hence relative errors in length measurements were estimated to be on the order of 2 x 10-4.
Two pressure transducers were employed for pressure measurements. The low-pressure transducer has a range of 0-7 atm (k0.3% full scale) and the high-pressureone has a range of 0-75 atm (*1.0% full scale). Sorption and dilation experimentswere performed at 25.0 "C in an air bath controlled to *0.5 "C.
Results and Discussion Sorption Isotherms. Sorption isotherms for five gases (C&, C3H8, n-CdHlo, is044H10, and n-CsH12) in the PB film were measured in this study. In the case of the EVAc film, sorption experiments were performed for all of the seven gases. Measurements on sorption and desorption runs for each gas were done stepwise up to the maximum pressure (0.4 to 40 atm) and then also stepwise down to vacuum mmHg). The sorption and desorption equilibria for all the gases were reached within a few hours. All sorption isotherms are presented in Figures 1 and 2. Some are depicted by solid curveswithout experimental points because of the simplicity of the figures, and only low-pressure parts of sorption isotherms are presented for gases with relatively low solubility. In the figures,sorption isotherms for C2H4 and C2H6 in PB and for CH4 in EVAc, which were reported in previous ~ a p e r s , are ~ J also shown. The isotherms, which are convex with respect to the pressure axis, are analyzed using a simplified equation for the Flory-Huggins dissolution. According to a derivation by Suwandi and Stern? concentration of a dissolved gas in a rubbery polymer is given by
C = k g exp(uC) (1) are the pressure, the Henry's law parameter, and the constant related to the polymer-
kD, and u
penetrant interaction, respectively. Dissolution parameters kD and u were estimated by fitting data using the equation In (Clp) = In k~ uC. The resulta are given in Tables I and I1 together with ranges of pressure used in the experiments. The dissolution parameters for CHI, C2H4, and C2H6 in PB and for CHI in EVAc are cited in the tables, for comparison, from the previous papers. The magnitude of errors in concentration determination for CH4 was in the range *l%to f4% and those for the others were less than *l%. Dilation Isotherms. Measurements of the length of the film, as well as sorption experiments, were performed stepwise up to the maximum pressure and then down to
OO24-9297/92/2225-4321$03.00/00 1992 American Chemical Society
4322 Kamiya et al.
Macromolecules, Vol. 25, No. 17, 1992
Table I1 Dissolution Parameters and Partial Molar Volumes for Gases in Poly(ethy1ene-cevinyl acetate) at 25 O C * range of gas
CHI CZH4 CZH6 C3H6 C3Hs n-C4Hl0 iso-CqH10 n-CsH12
50 7 7 5 5 0.8 1.5 0.4
0.145 0.634 0.843 2.86 2.80 9.32 5.78 29.76
x 103 8.5 10.5 12.7 14.3 19.7 19.7 20.9
46 f 1 61.0 f 1.0 64.9 i 0.6 73.7 f0.4 79.3 i 0.4 93.8 f 1.0 102.1 f 1.0 106.9 f 0.9
See footnote a in Table I for units.
Figure 1. Sorption isotherms for organic gases in polybutadiene at 25.0 "C. CzHd and C2HB isotherms are earlier data.5 Open
and solid symbols correspond to sorption and desorption runs, respectively, throughout this paper.
c. CC(STP)/CC(poIym) Figure 3. Elongation plotted versus concentration for organic gases in polybutadiene. C&, C2H4, and C2H$ isothermsare earlier
Figure 2. Sorptionisothermsfor organicgases in poly(ethy1eneco-vinyl acetate) at 25 "C. CHI isotherm is earlier d a h 7 Table I Dissolution Parameters and Partial Molar Volumes for Gases in Polybutadiene at 25 O C . range of gas pressure(atm) kD u x 103 VR ref 44 f 1 5 CH4 50 0.226 40 1.18 3.1 52.0 f 0.5 5 C2H4 20 1.82 3.6 57.0 f 0.5 5 C2H6 8.0 71.8 f 0.4 C3H6 7 5.09 7.8 79.8 f 1.2 C3He 7 4.97 12.8 95.2 f 0.6 n-C4H10 0.9 16.52 2 10.31 13.6 96.1 f 1.1 iso-C4Hlo 13.9 106.1 f 1.5 n-C5HlZ 0.5 51.67 0 Unite: k ~cm3(STP)/(cm3(polym) , a h ) ; u, cm3(polym)/cm3(STP); VR,cm3/mol.
vacuum. Dilation isotherms in the form of elongation versus pressure for the gases are very similar in shape to the corresponding sorption isotherms. The elongation is defined as 1, = ( L - Lo)/Lo,where L is the length a t p ( C ) and LOthe length a t p = 0 (C = 0). In Figures 3 and 4, the elongation data are plotted as a function of concentration. Earlier data for CHI, C2H4, and C2Hs in PB and for CHI in EVAc are also shown in the figures.537 Some data are depicted by solid curves without experimental
c , CC(STP)/CC(polym) Figure 4. Elongation plotted versus concentration for gases in poly(ethy1ene-co-vinyl acetate). CHI isotherm is earlier d a h 7
points because of the simplicity of the figures. As shown in the figures, each plot is linear except for that of the PB film in the high-elongation region. The dilation isotherm obtained on the sorption run for every gas coincides with that on the desorption run. This indicates that creeping flow of the film specimen does not occur in dilation experiments. Hence the elongation data may be used as equilibrium values to characterize the total volume dilation. Experimental points for the PB film deviate slightly and negatively from linearity a t low concentration as the
Macromolecules, Val. 25, No. 17, 1992
Organic Gases in Rubbery Polymers 4323
elongation exceeds ca. 4 X This elongation corresponds nearly to a volume dilation of 12 vol 9%. Considering that the partial molar volume must remain nearly constant in the small ranges of concentration studied here, such concavity of the I, vs C plot at high concentrations may be due to a break in the isotropy of the film dilation; that is, length elongation in the plane directions of the film seems to become smaller than a fractional increase in ita thickness when the polymer swells by more than 12 vol % . Pope et al., however, reported that a siliconerubber film undergoes an isotropic dilation up to an elongation during sorption of high pressure C02.9 of at least 9 X At the present time, no reasonable explanation can be offered for the difference between PB and silicone rubber films. Partial Molar Volumes. The partial molar volume of a gas in a rubbery polymer can be obtained from sorption and elongation data, because the gas sorption is usually restricted to very low concentration^.^^^ When the dilation is assumed to be isotropic and the compression of the polymer by a hydrostatic component of the gas pressure is negligible, the partial molar volume is given as
Figure 5. Correlations of partial molar volume with van der Waals volume for gases in (0)polybutadiene and (A) poly(ethylene-co-vinyl acetate), where solid symbols belong to isoC4HI0.Dotted line is molar volume plotted versus van der Waals volume for liquid n-alkanes (carbon number 5-24) at 20 O C .
3 X 22410(dl,/dC)
where V is the volume of the polymer-gas mixture containing N moles of polymer and n moles of gas, and the volumetric concentration C is equal to 22410n/ V cm3(STP)/ cm3(polym). As shown above, each dilation isotherm plotted in the form of elongation versus concentration exhibits a straight line except for the high-elongation region (Figures 3 and 4). From linear parts of the isotherms, partial molar volumes of the dissolved organic gases were calculated according to eq 3. Results are presented in Tables I and 11together with earlier Relative errors in the VR determination by a least-squares method are within f1.5 % as listed in the tables. In a case of a sparingly soluble gas (such as CH4) whose value of k~ is muchsmaller than 1 (cm3(STP)/cm3(polym))/ atm, the hydrostatic compression of the polymer by pressure of the gas is not negligibly small compared with the sorptive dilation. A partial molar volume of such a gas is approximately given by VR = 22410 d[31, + &p]/ dC, where BT is the compressibility of the penetrant-free polymere5The CH4 data in Figures 3 and 4 are therefore plotted in the form of (1, + @Tp/3)versus concentration, atm-l for PB and 3.9 where values of BT are 4.75 X X atm-l for EVAc. The partial molar volumes thus obtained are cited in Tables I and I1from the earlier papers. Relation between Partial Molar Volume and Molecular Size. Figure 5 shows partial molar volumes plotted versus van der Waals volumes VW for the eight organic gases. The van der Waals volumes used here were calculated according to a group contribution method by Bondi.lO The linear relationship found in the range of elongation below 4 X or of concentration below 30-40 cm3(STP)/cm3(polym)is expressed as
vR = 1.6Vw + 18.5 cm3/mol The relation agreesvery closely with a relationship between molar volume and van der Waals volume for liquid nalkanes (carbon number n = 5-24); P = 1.59vw + 21.41 in cm3/mol at 20 O C . I 1 The latter is also shown as a dotted line in Figure 5.
Figure 6. Flory-Huggins parameter plotted versus van der Waals volume: (0) n-alkanes; (A)iso-C4Hlo;(0)n-alkenes.
This result indicates that an additivity rule holds for the partial molar volumes of the dissolved gases, as well as for their van der Waals volumes.10J2 We then tried to divide the partial molar volumes of the n-alkane gases into contributions of the methylene group V(CH2) and methyl group V(CH3) to itself and had the linear relation between thepartial molar volume and carbon number n; VR = (n- 2)V(CH2) + 2V(CH3), where V(CH2) = 16 cm3/ mol and V(CH3) = 31 cm3/mol. These contributions are almost the same as those for the molar volumes of the liquid n-alkanes, i.e., V(CH2) = 16.3 cm3/mol and V(CH3) = 32.5 cm3/mol. From the above results, it is inferred that gas molecules dissolved in the polymers are in almost the same thermodynamic state as molecules of liquid in itself are. Interaction between Polymer and Gas. The FloryHuggins parameter x was estimated from the values of Q and VR using the relation u = 2(1+ x ) v ~ / 2 2 4 1 0 .Results ~ are presented as a function of van der Waals volume in Figure 6. According to the definition, the quantity of x multiplied by the Boltzmann constant and temperature is equivalent to the difference in energy of a gas molecule inserted in the pure polymer compared with one in its own 1 i q ~ i d . IThe ~ value of x for a homologous series of organic gases is therefore expected to vary in proportion to molecular size or carbon number. The data shown in Figure
Macromolecules, Vol. 25, No. 17, 1992
4324 Kamiya et al.
6 agree well with this expectation. The values of x for C2H4 and C & j in PB, however, became negative. The cause of the negative values is not clear, but it may be partly related to the fact that the dissolution studied here is not an isobaric process. That is, because the Flory-Huggins equation is a solution theory of a polymer-solvent system at constant temperature and pressure, it is not applicable to the gas dissolution of a polymer in which the effect of the hydrostatic component of the gas pressure on its solubility is not negligibly small. Therefore we compensated amounts of the dissolved gases for their decreases in solubility due to pressure using the relation (a In L , / a p ) =~ / 3 -~ VR/RT,where L, is the Ostwald coefficient of solubility.14 The corrected amounts of the dissolved gases, which can be regarded as isobaric values at 1 atm, were again analyzed by the abovementioned method. However,reestimated values of x were still negative, but came close to zero; x = -0.1 for both C2H4 and C&. There will possibly be other causes to get x negative such as thermal behavior of the dissolution and experimental errors in pressure measurements. Comparison among the Two Polymers and Others. As shown in Tables I and 11,the solubilities of PB to the organic gases are about twice those of EVAc, which are similar in magnitude to the solubilities of low-density p01yethylene.l~ Since the degrees of crystallinity of the polymers are much the same (PB, 0.26; EVAc, 0.3), it is apparent that the organic gases have better affinities for PB molecules than EVAc molecules. This tendency is consistent with the result shown in Figure 6 that x values of PB are much smaller than those of EVAc. For C3H8 and C4H10, the x values of PB obtained in this study are comparable to those of natural rubber estimated by van Amerongen.' The partial molar volumes of the organic gases in the two polymers are almost the same, as shown in Tables I and I1 and in Figure 5. By comparing these volumes with literature data for other polymers, it can be confirmed whether the linear relation between the partial molar volume and the van der Waals volume found in this study is accepted as a general rule. However, there are only a few data of VR available for comparison: CH4 41, CzH4 55.2, and C2H6 56.0 cm3/mol in a poly(dimethylsi1oxane) rubber at 25 'C;l6 C2H4 52, C& 65, and C3H8 77 cm3/mol in poly(ethy1 methacrylate) above the glass transition concentration at 15 OC;17 CHI 52.2, C2H2 50.4, C2H4 61.0, and C2H6 67.1 cm3/mol on the average in five organic solvents (carbon tetrachloride, chlorobenzene, benzene, acetone, and methyl acetate) at 25 OC.18 In spite of the large differences in solubilities, the partial molar volumes in these polymers and the organic solvents are very similar in magnitude to the values obtained here and have also a tendency to increase with size of the gas molecule. Furthermore, the linear relation found here is almost the same as that between the molar volume and the van der Waals volume for a series of liquid n-alkanes,as mentioned above. From these facts, it may be concluded that the linearity of partial molar volume versus van der Waals volume existsin nearly every system consistingof a rubbery
polymer and a homologous series of organic gases. Conclusions Sorption isotherms for organic gases in two rubbery polymers, 1,2-polybutadiene and poly(ethy1ene-co-vinyl acetate), are well described as the Flory-Huggins dissolution. Dilation isotherms in the form of elongation versus pressure mimic the corresponding sorption isotherms. Plotting elongation versus concentration gives a linearity except for the high-concentration region. Partial molar volumes of dissolved organic gases are determined from sorption and elongation data, and a linear relation is found between the volumes and the van der Waals volumes. The linear relation, which is similar to that between the molar volume and the van der Waals volume for liquid n-alkanes, will possibly exist in every rubbery polymer-organic gas system. The present data at relatively low concentrations make it possible to conclude that the additivity rule of partial molar volume is obeyed by organic gases dissolved in rubbery polymers and that the dissolved molecules are in almost the same thermodynamic state as molecules of liquid in itself are. The results will give us the volumetric approach, one of the most fundamental approaches, to the understanding of every phenomenon or process relating to polymer-gas systems such as sorption, diffusion, and permeation of gases in rubbery polymers and plasticization of polymers due to sorption of gases. References and Notes van Amerongen, G. J. J. Polym. Sei. 1960,5,307. Fleming, G . K.; Koros, W. J. Macromolecules 1986, 19, 2285. Hirose, T.;Mizoguchi, K.; Kamiya, Y. J. Polym. Sci., Part B Polym. Phys. 1986,24, 2107. Kamiya, Y.; Hirose, T.;Naito, Y.; Mizoguchi, K. J. Polym. Sci., Part B Polym. Phys. 1989,27, 879. Kamiya, Y.; Naito, Y.; Mizoguchi, K. J. Polym. Sci., Part B Polym. Phys. 1989, 27, 2243. Briscoe, B. J.; Zakaria, S. J. Polym. Sci., Part B Polym. Phys. 1991, 29, 989. Kamiya, Y.; Naito,Y.; Bourbon, D., to be published. Suwandi, M. S.; Stern, S. A. J. Polym. Sci., Polym. Phys. Ed. 1973, 11,663. Pope, D. S.;Koros, W. J.; Fleming, G. K. J. Polym. Sci., Part B: Polym. Phys. 1989,27, 1173. Bondi, A. J . Phys. Chem. 1964,68,441. Lide, D. R., Ed.CRC Handbook of Chemistry andPhysics, 71st ed.; CRC Press: Boca Raton, FL, 1990. Yoshimura, Y.; Nakahara, M. Ber. Bunsenges. Phys. Chem. 1985,89, 25, 426. Flory, P. J. Principles ofpolymerChemistry;Comell University Press: Ithaca, NY, 1953. Horiuti, J. Textbook of Chemical Thermodynamics; Kodansha: Tokyo, 1981. Michaels, A. S.; Bixler, H. J. J. Polym. Sci. 1961,50, 413. Kamiya, Y.; Natio, Y.; Hirose, T.;Mizoguchi, K. J. Polym. Sci., Part B: Polym. Phys. 1990,223, 1297. Kamiya, Y.; Bourbon, D.; Mizoguchi, K.; Naito, Y. Polym. J. 1992, 24, 445. Horiuti, J. Sci. Pap. Inst. Phys. Chem. Res. Tokyo 1931, 17, 125.
Registry No. C2H2, 74-85-1; C2H6, 74-84-0; C&, 115-07-1; C ~ H B74-98-6; , n-CbHlo,106-97-8;iso-CdHlo,75-28-5; n-CaHlp, 10966-0; (ethylene)(vinyl acetate) (copolymer), 24937-78-8.